# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.
# This journal is © The Royal Society of Chemistry 2017

 
data_shelx
 
_audit_creation_method            'SHELXL-97'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          
 'Al2 O32 P9 V2, 7(Na)'
_chemical_formula_sum
 'Al2 Na7 O32 P9 V2' 
_chemical_formula_weight          1107.50

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Al'  'Al'   0.0645   0.0514
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'V'  'V'   0.3005   0.5294
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       tetragonal
_space_group_IT_number            114
_space_group_name_H-M_alt         'P -4 21 c'
_space_group_name_Hall            'P -4 2n'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x, -y, z'
 'y, -x, -z'
 '-y, x, -z'
 '-x+1/2, y+1/2, -z+1/2'
 'x+1/2, -y+1/2, -z+1/2'
 '-y+1/2, -x+1/2, z+1/2'
 'y+1/2, x+1/2, z+1/2'
 
_cell_length_a                    14.109(3)
_cell_length_b                    14.109(3)
_cell_length_c                    6.2483(13)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      1243.8(6)
_cell_formula_units_Z             2
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     1044
_cell_measurement_theta_min       2.88
_cell_measurement_theta_max       23.74
 
_exptl_crystal_description        'needle' 
_exptl_crystal_colour             'yellow'
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     2.957          
_exptl_crystal_F_000              1080
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.04
_exptl_crystal_size_mid           0.01
_exptl_crystal_size_min           0.01 
_exptl_absorpt_coefficient_mu     1.672
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type    'multi-scan'
_exptl_absorpt_correction_T_min   0.5585
_exptl_absorpt_correction_T_max   0.7461
_exptl_absorpt_process_details    'Bruker SADABS'
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'fine-focus sealed tube'  
_diffrn_measurement_device_type   'PHOTON 100 CMOS'
_diffrn_measurement_method        'φ and ω scans'
_diffrn_detector_area_resol_mean  ?
_diffrn_reflns_number             2248
_diffrn_reflns_av_unetI/netI      0.1540
_diffrn_reflns_av_R_equivalents   0.0928
_diffrn_reflns_limit_h_min        -18
_diffrn_reflns_limit_h_max        12
_diffrn_reflns_limit_k_min        -18
_diffrn_reflns_limit_k_max        4
_diffrn_reflns_limit_l_min        -6
_diffrn_reflns_limit_l_max        8
_diffrn_reflns_theta_min          3.566
_diffrn_reflns_theta_max          30.553
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.793
_diffrn_measured_fraction_theta_full  0.789
_diffrn_reflns_Laue_measured_fraction_max    0.793
_diffrn_reflns_Laue_measured_fraction_full   0.789
_diffrn_reflns_point_group_measured_fraction_max   0.846
_diffrn_reflns_point_group_measured_fraction_full  0.851
_reflns_number_total              1141
_reflns_number_gt                 759
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.845
_reflns_Friedel_fraction_max      0.919
_reflns_Friedel_fraction_full     0.941
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        'Bruker APEX3'
_computing_cell_refinement        'Bruker SAINT'
_computing_data_reduction         'Bruker SAINT'
_computing_structure_solution     'Superflip (Palatinus & Chapuis, 2007)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 97)'
_computing_molecular_graphics     'ATOMS (Dowty, 2002)'
_computing_publication_material   ?
_refine_special_details
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0217P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_extinction_coef        0.0010(6)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack    0.29(12)
_chemical_absolute_configuration  ?
_refine_ls_number_reflns          1141
_refine_ls_number_parameters      120
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.1180
_refine_ls_R_factor_gt            0.0642
_refine_ls_wR_factor_ref          0.0855
_refine_ls_wR_factor_gt           0.0757
_refine_ls_goodness_of_fit_ref    1.024
_refine_ls_restrained_S_all       1.024
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
V1 V 0.81818(16) 0.12135(17) 0.1333(2) 0.0095(5) Uani 0.5 1 d . . P . .
Al1 Al 0.81818(16) 0.12135(17) 0.1333(2) 0.0095(5) Uani 0.5 1 d . . P . .
P1 P 0.0000 0.0000 0.0000 0.0068(12) Uani 1 4 d S T P . .
P2 P 0.6239(2) 0.2570(2) 0.1458(3) 0.0078(6) Uani 1 1 d . . . . .
P3 P 0.95804(19) 0.30135(19) 0.1052(3) 0.0090(6) Uani 1 1 d . . . . .
Na1 Na 0.0000 0.0000 0.5000 0.055(4) Uani 1 4 d S T P . .
Na2 Na 0.0000 0.5000 0.8213(6) 0.0310(19) Uani 1 2 d S T P . .
Na3 Na 0.9197(3) 0.2585(3) 0.5988(5) 0.0240(12) Uani 1 1 d . . . . .
O1 O 0.1371(5) 0.1706(6) 0.1807(7) 0.016(2) Uani 1 1 d . . . . .
O2 O 0.7032(5) 0.1914(5) 0.1133(8) 0.0194(19) Uani 1 1 d . . . . .
O3 O 0.9326(5) 0.0533(5) 0.1488(8) 0.0131(17) Uani 1 1 d . . . . .
O4 O 0.5373(5) 0.1890(6) 0.2104(8) 0.0174(19) Uani 1 1 d . . . . .
O5 O 0.5913(6) 0.3071(5) 0.9431(7) 0.018(2) Uani 1 1 d . . . . .
O6 O 0.0067(5) 0.2558(5) 0.9148(7) 0.0130(17) Uani 1 1 d . . . . .
O7 O 0.9278(5) 0.4004(5) 0.0669(7) 0.0117(18) Uani 1 1 d . . . . .
O8 O 0.8813(7) 0.2410(6) 0.2020(8) 0.022(2) Uani 1 1 d . . . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
V1 O3 1.881(7) . ?
V1 O2 1.904(7) . ?
V1 O6 1.948(8) 4_656 ?
V1 O8 1.956(8) . ?
V1 O1 1.981(5) 4_655 ?
V1 O5 1.987(5) 8_544 ?
V1 O4 3.422(6) 8_544 ?
V1 Na3 3.474(5) 4_646 ?
V1 O6 3.540(7) 1_654 ?
V1 O3 3.672(7) 4_645 ?
V1 O2 3.678(6) 8_545 ?
P1 O3 1.528(6) 4_545 ?
P1 O3 1.528(6) 2_655 ?
P1 O3 1.528(6) 3_565 ?
P1 O3 1.528(6) 1_455 ?
P1 Na1 3.1241(6) . ?
P1 Na1 3.1241(6) 1_554 ?
P1 O1 3.288(8) . ?
P1 O1 3.288(8) 2 ?
P1 O1 3.288(8) 4 ?
P1 O1 3.288(8) 3 ?
P2 O2 1.466(7) . ?
P2 O1 1.502(7) 6 ?
P2 O5 1.521(6) 1_554 ?
P2 O4 1.605(7) . ?
P2 Na3 2.993(5) 8_544 ?
P2 O2 3.165(5) 8_545 ?
P2 O6 3.211(6) 6_556 ?
P2 Na3 3.269(5) 6_455 ?
P2 O2 3.543(6) 8_544 ?
P2 O8 3.553(9) 6_455 ?
P3 O7 1.481(7) . ?
P3 O8 1.504(8) . ?
P3 O6 1.516(6) 1_654 ?
P3 O4 1.612(6) 6 ?
P3 O1 3.163(8) 1_655 ?
P3 Na2 3.167(3) 7_654 ?
P3 Na3 3.189(4) . ?
P3 Na3 3.267(4) 1_554 ?
P3 Na3 3.274(6) 8_544 ?
P3 Na2 3.369(3) 1_654 ?
P3 O1 3.443(7) 4_655 ?
P3 O7 3.488(6) 8_545 ?
Na1 O3 2.507(6) 3_566 ?
Na1 O3 2.507(6) 1_455 ?
Na1 O3 2.507(6) 2_655 ?
Na1 O3 2.507(6) 4_546 ?
Na1 O5 3.033(8) 6_456 ?
Na1 O5 3.033(8) 5_546 ?
Na1 O5 3.033(8) 8_444 ?
Na1 O5 3.033(8) 7_554 ?
Na1 P1 3.1241(6) 1_556 ?
Na1 O1 3.676(7) . ?
Na1 O1 3.676(7) 2 ?
Na2 O7 2.317(7) 2_666 ?
Na2 O7 2.317(7) 1_456 ?
Na2 O7 2.354(6) 8_445 ?
Na2 O7 2.354(6) 7_565 ?
Na2 O4 2.725(8) 4_556 ?
Na2 O4 2.725(8) 3_566 ?
Na2 Na2 3.1241(6) 7_554 ?
Na2 Na2 3.1242(6) 7 ?
Na2 P3 3.167(3) 8_445 ?
Na2 P3 3.167(3) 7_565 ?
Na2 P3 3.369(3) 2_666 ?
Na2 P3 3.369(3) 1_456 ?
Na3 O6 2.325(7) 1_655 ?
Na3 O7 2.412(9) 8_545 ?
Na3 O1 2.541(8) 4_656 ?
Na3 O8 2.550(6) . ?
Na3 O5 2.606(9) 6_556 ?
Na3 O4 2.653(8) 6 ?
Na3 P2 2.993(5) 8_545 ?
Na3 O5 3.005(9) 8_544 ?
Na3 O8 3.127(10) 8_545 ?
Na3 P3 3.267(4) 1_556 ?
Na3 P2 3.269(5) 6 ?
O1 P2 1.502(7) 6_455 ?
O1 Al1 1.981(5) 3_565 ?
O1 V1 1.981(5) 3_565 ?
O1 O5 2.458(6) 6_456 ?
O1 O2 2.514(10) 6_455 ?
O1 O4 2.524(10) 6_455 ?
O1 Na3 2.540(8) 3_566 ?
O1 O2 2.671(9) 3_565 ?
O1 O6 2.755(9) 1_554 ?
O1 O3 2.785(9) 3_565 ?
O1 O8 2.898(8) 3_565 ?
O1 O6 3.068(10) 3_556 ?
O2 O4 2.418(10) . ?
O2 O5 2.507(10) 1_554 ?
O2 O1 2.513(10) 6 ?
O2 O8 2.667(12) . ?
O2 O1 2.671(9) 4_655 ?
O2 O6 2.676(10) 4_656 ?
O2 O5 2.896(9) 8_544 ?
O2 O2 3.1330(13) 8_545 ?
O2 O2 3.1330(13) 8_544 ?
O3 P1 1.528(6) 1_655 ?
O3 O3 2.425(14) 2_755 ?
O3 Na1 2.507(6) 1_655 ?
O3 O3 2.530(10) 3_665 ?
O3 O3 2.530(10) 4_645 ?
O3 O5 2.609(8) 8_544 ?
O3 O8 2.764(11) . ?
O3 O6 2.767(10) 4_656 ?
O3 O1 2.785(9) 4_655 ?
O3 O1 3.315(10) 2_655 ?
O4 P3 1.612(6) 6_455 ?
O4 O7 2.432(9) 6_455 ?
O4 O8 2.474(13) 6_455 ?
O4 O5 2.479(9) 1_554 ?
O4 O6 2.506(7) 6_556 ?
O4 O1 2.524(10) 6 ?
O4 Na3 2.653(8) 6_455 ?
O4 Na2 2.725(8) 3_556 ?
O4 O7 3.074(9) 3_565 ?
O4 O2 3.332(9) 8_545 ?
O5 P2 1.521(6) 1_556 ?
O5 V1 1.987(5) 8_545 ?
O5 Al1 1.987(5) 8_545 ?
O5 O1 2.458(6) 6_556 ?
O5 O4 2.479(9) 1_556 ?
O5 O2 2.507(10) 1_556 ?
O5 Na3 2.606(9) 6_456 ?
O5 O3 2.609(8) 8_545 ?
O5 O6 2.686(8) 6_556 ?
O5 O8 2.797(11) 8_545 ?
O5 O2 2.896(9) 8_545 ?
O5 Na3 3.005(9) 8_545 ?
O6 P3 1.516(6) 1_456 ?
O6 Al1 1.948(8) 3_566 ?
O6 V1 1.948(8) 3_566 ?
O6 Na3 2.325(7) 1_455 ?
O6 O4 2.506(7) 6_456 ?
O6 O7 2.512(10) 1_456 ?
O6 O8 2.528(10) 1_456 ?
O6 O2 2.676(10) 3_566 ?
O6 O5 2.686(8) 6_456 ?
O6 O1 2.755(9) 1_556 ?
O6 O3 2.767(10) 3_566 ?
O6 O1 3.068(10) 4_556 ?
O7 Na2 2.317(7) 1_654 ?
O7 Na2 2.354(6) 7_654 ?
O7 Na3 2.412(9) 8_544 ?
O7 O4 2.432(9) 6 ?
O7 O8 2.491(11) . ?
O7 O6 2.512(10) 1_654 ?
O7 O4 3.073(9) 4_655 ?
O7 O7 3.171(3) 8_544 ?
O7 O7 3.171(3) 8_545 ?
O7 O7 3.471(15) 2_765 ?
O7 P3 3.488(6) 8_544 ?
O8 O4 2.474(13) 6 ?
O8 O6 2.528(10) 1_654 ?
O8 O5 2.797(11) 8_544 ?
O8 O1 2.898(8) 4_655 ?
O8 Na3 3.127(10) 8_544 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O3 V1 O2 179.0(3) . . ?
O3 V1 O6 92.5(3) . 4_656 ?
O2 V1 O6 88.0(3) . 4_656 ?
O3 V1 O8 92.2(4) . . ?
O2 V1 O8 87.4(4) . . ?
O6 V1 O8 173.8(3) 4_656 . ?
O3 V1 O1 92.3(3) . 4_655 ?
O2 V1 O1 86.8(3) . 4_655 ?
O6 V1 O1 89.0(3) 4_656 4_655 ?
O8 V1 O1 94.8(3) . 4_655 ?
O3 V1 O5 84.8(3) . 8_544 ?
O2 V1 O5 96.2(3) . 8_544 ?
O6 V1 O5 86.0(3) 4_656 8_544 ?
O8 V1 O5 90.4(3) . 8_544 ?
O1 V1 O5 174.1(4) 4_655 8_544 ?
O3 V1 O4 108.7(2) . 8_544 ?
O2 V1 O4 71.1(2) . 8_544 ?
O6 V1 O4 46.21(19) 4_656 8_544 ?
O8 V1 O4 135.3(2) . 8_544 ?
O1 V1 O4 46.9(2) 4_655 8_544 ?
O5 V1 O4 129.5(3) 8_544 8_544 ?
O3 V1 Na3 79.9(2) . 4_646 ?
O2 V1 Na3 101.1(2) . 4_646 ?
O6 V1 Na3 39.42(17) 4_656 4_646 ?
O8 V1 Na3 137.98(19) . 4_646 ?
O1 V1 Na3 126.4(2) 4_655 4_646 ?
O5 V1 Na3 48.1(2) 8_544 4_646 ?
O4 V1 Na3 85.55(13) 8_544 4_646 ?
O3 V1 O6 69.4(2) . 1_654 ?
O2 V1 O6 109.7(3) . 1_654 ?
O6 V1 O6 142.0(2) 4_656 1_654 ?
O8 V1 O6 44.0(2) . 1_654 ?
O1 V1 O6 59.9(2) 4_655 1_654 ?
O5 V1 O6 123.3(2) 8_544 1_654 ?
O4 V1 O6 106.73(14) 8_544 1_654 ?
Na3 V1 O6 149.15(16) 4_646 1_654 ?
O3 V1 O3 39.7(3) . 4_645 ?
O2 V1 O3 140.0(2) . 4_645 ?
O6 V1 O3 65.7(2) 4_656 4_645 ?
O8 V1 O3 120.4(3) . 4_645 ?
O1 V1 O3 64.3(2) 4_655 4_645 ?
O5 V1 O3 110.6(3) 8_544 4_645 ?
O4 V1 O3 68.96(18) 8_544 4_645 ?
Na3 V1 O3 77.94(14) 4_646 4_645 ?
O6 V1 O3 80.35(16) 1_654 4_645 ?
O3 V1 O2 122.39(19) . 8_545 ?
O2 V1 O2 58.42(14) . 8_545 ?
O6 V1 O2 97.2(2) 4_656 8_545 ?
O8 V1 O2 76.8(2) . 8_545 ?
O1 V1 O2 144.2(3) 4_655 8_545 ?
O5 V1 O2 40.0(3) 8_544 8_545 ?
O4 V1 O2 118.65(19) 8_544 8_545 ?
Na3 V1 O2 73.32(14) 4_646 8_545 ?
O6 V1 O2 120.77(17) 1_654 8_545 ?
O3 V1 O2 149.23(16) 4_645 8_545 ?
O3 P1 O3 111.7(2) 4_545 2_655 ?
O3 P1 O3 105.0(4) 4_545 3_565 ?
O3 P1 O3 111.7(2) 2_655 3_565 ?
O3 P1 O3 111.7(2) 4_545 1_455 ?
O3 P1 O3 105.0(4) 2_655 1_455 ?
O3 P1 O3 111.7(2) 3_565 1_455 ?
O3 P1 Na1 127.5(2) 4_545 . ?
O3 P1 Na1 52.5(2) 2_655 . ?
O3 P1 Na1 127.5(2) 3_565 . ?
O3 P1 Na1 52.5(2) 1_455 . ?
O3 P1 Na1 52.5(2) 4_545 1_554 ?
O3 P1 Na1 127.5(2) 2_655 1_554 ?
O3 P1 Na1 52.5(2) 3_565 1_554 ?
O3 P1 Na1 127.5(2) 1_455 1_554 ?
Na1 P1 Na1 180.0 . 1_554 ?
O3 P1 O1 162.6(2) 4_545 . ?
O3 P1 O1 77.6(3) 2_655 . ?
O3 P1 O1 57.6(2) 3_565 . ?
O3 P1 O1 78.3(3) 1_455 . ?
Na1 P1 O1 69.92(9) . . ?
Na1 P1 O1 110.08(9) 1_554 . ?
O3 P1 O1 57.6(2) 4_545 2 ?
O3 P1 O1 78.3(3) 2_655 2 ?
O3 P1 O1 162.6(2) 3_565 2 ?
O3 P1 O1 77.6(3) 1_455 2 ?
Na1 P1 O1 69.92(9) . 2 ?
Na1 P1 O1 110.08(9) 1_554 2 ?
O1 P1 O1 139.84(18) . 2 ?
O3 P1 O1 78.3(3) 4_545 4 ?
O3 P1 O1 162.6(2) 2_655 4 ?
O3 P1 O1 77.6(3) 3_565 4 ?
O3 P1 O1 57.6(2) 1_455 4 ?
Na1 P1 O1 110.08(9) . 4 ?
Na1 P1 O1 69.92(9) 1_554 4 ?
O1 P1 O1 96.77(6) . 4 ?
O1 P1 O1 96.77(6) 2 4 ?
O3 P1 O1 77.6(3) 4_545 3 ?
O3 P1 O1 57.6(2) 2_655 3 ?
O3 P1 O1 78.3(3) 3_565 3 ?
O3 P1 O1 162.6(2) 1_455 3 ?
Na1 P1 O1 110.08(9) . 3 ?
Na1 P1 O1 69.92(9) 1_554 3 ?
O1 P1 O1 96.77(6) . 3 ?
O1 P1 O1 96.77(6) 2 3 ?
O1 P1 O1 139.84(18) 4 3 ?
O2 P2 O1 115.8(4) . 6 ?
O2 P2 O5 114.1(4) . 1_554 ?
O1 P2 O5 108.8(4) 6 1_554 ?
O2 P2 O4 103.8(4) . . ?
O1 P2 O4 108.6(3) 6 . ?
O5 P2 O4 104.9(4) 1_554 . ?
O2 P2 Na3 89.2(3) . 8_544 ?
O1 P2 Na3 58.0(3) 6 8_544 ?
O5 P2 Na3 75.8(3) 1_554 8_544 ?
O4 P2 Na3 165.0(3) . 8_544 ?
O2 P2 O2 75.33(19) . 8_545 ?
O1 P2 O2 57.3(3) 6 8_545 ?
O5 P2 O2 166.1(4) 1_554 8_545 ?
O4 P2 O2 81.6(3) . 8_545 ?
Na3 P2 O2 94.79(18) 8_544 8_545 ?
O2 P2 O6 118.4(3) . 6_556 ?
O1 P2 O6 59.0(3) 6 6_556 ?
O5 P2 O6 125.6(4) 1_554 6_556 ?
O4 P2 O6 50.1(2) . 6_556 ?
Na3 P2 O6 116.98(16) 8_544 6_556 ?
O2 P2 O6 49.63(17) 8_545 6_556 ?
O2 P2 Na3 124.5(3) . 6_455 ?
O1 P2 Na3 119.5(3) 6 6_455 ?
O5 P2 Na3 51.4(3) 1_554 6_455 ?
O4 P2 Na3 53.6(3) . 6_455 ?
Na3 P2 Na3 124.37(17) 8_544 6_455 ?
O2 P2 Na3 132.90(16) 8_545 6_455 ?
O6 P2 Na3 86.67(15) 6_556 6_455 ?
O2 P2 O2 61.9(2) . 8_544 ?
O1 P2 O2 142.3(3) 6 8_544 ?
O5 P2 O2 53.1(3) 1_554 8_544 ?
O4 P2 O2 108.2(3) . 8_544 ?
Na3 P2 O2 84.36(15) 8_544 8_544 ?
O2 P2 O2 137.3(3) 8_545 8_544 ?
O6 P2 O2 158.4(2) 6_556 8_544 ?
Na3 P2 O2 77.51(14) 6_455 8_544 ?
O2 P2 O8 141.0(4) . 6_455 ?
O1 P2 O8 85.4(3) 6 6_455 ?
O5 P2 O8 85.9(3) 1_554 6_455 ?
O4 P2 O8 37.3(3) . 6_455 ?
Na3 P2 O8 129.13(18) 8_544 6_455 ?
O2 P2 O8 92.56(17) 8_545 6_455 ?
O6 P2 O8 43.53(16) 6_556 6_455 ?
Na3 P2 O8 43.65(11) 6_455 6_455 ?
O2 P2 O8 120.81(17) 8_544 6_455 ?
O7 P3 O8 113.1(5) . . ?
O7 P3 O6 113.8(4) . 1_654 ?
O8 P3 O6 113.6(4) . 1_654 ?
O7 P3 O4 103.6(4) . 6 ?
O8 P3 O4 105.1(5) . 6 ?
O6 P3 O4 106.4(4) 1_654 6 ?
O7 P3 O1 143.6(3) . 1_655 ?
O8 P3 O1 100.6(4) . 1_655 ?
O6 P3 O1 60.5(3) 1_654 1_655 ?
O4 P3 O1 52.3(3) 6 1_655 ?
O7 P3 Na2 44.6(2) . 7_654 ?
O8 P3 Na2 117.7(3) . 7_654 ?
O6 P3 Na2 128.7(3) 1_654 7_654 ?
O4 P3 Na2 59.4(3) 6 7_654 ?
O1 P3 Na2 107.65(15) 1_655 7_654 ?
O7 P3 Na3 106.6(2) . . ?
O8 P3 Na3 51.8(3) . . ?
O6 P3 Na3 139.0(3) 1_654 . ?
O4 P3 Na3 56.1(3) 6 . ?
O1 P3 Na3 83.15(12) 1_655 . ?
Na2 P3 Na3 77.71(12) 7_654 . ?
O7 P3 Na3 88.3(2) . 1_554 ?
O8 P3 Na3 99.5(3) . 1_554 ?
O6 P3 Na3 40.2(3) 1_654 1_554 ?
O4 P3 Na3 145.4(3) 6 1_554 ?
O1 P3 Na3 99.72(14) 1_655 1_554 ?
Na2 P3 Na3 127.44(13) 7_654 1_554 ?
Na3 P3 Na3 150.87(17) . 1_554 ?
O7 P3 Na3 43.0(3) . 8_544 ?
O8 P3 Na3 71.0(4) . 8_544 ?
O6 P3 Na3 126.6(3) 1_654 8_544 ?
O4 P3 Na3 124.2(3) 6 8_544 ?
O1 P3 Na3 170.42(14) 1_655 8_544 ?
Na2 P3 Na3 73.42(10) 7_654 8_544 ?
Na3 P3 Na3 87.85(12) . 8_544 ?
Na3 P3 Na3 86.56(12) 1_554 8_544 ?
O7 P3 Na2 35.0(3) . 1_654 ?
O8 P3 Na2 144.0(4) . 1_654 ?
O6 P3 Na2 82.0(3) 1_654 1_654 ?
O4 P3 Na2 100.6(3) 6 1_654 ?
O1 P3 Na2 115.04(15) 1_655 1_654 ?
Na2 P3 Na2 57.01(5) 7_654 1_654 ?
Na3 P3 Na2 134.16(13) . 1_654 ?
Na3 P3 Na2 70.93(11) 1_554 1_654 ?
Na3 P3 Na2 73.77(9) 8_544 1_654 ?
O7 P3 O1 113.5(3) . 4_655 ?
O8 P3 O1 56.5(3) . 4_655 ?
O6 P3 O1 63.0(3) 1_654 4_655 ?
O4 P3 O1 142.5(4) 6 4_655 ?
O1 P3 O1 96.1(3) 1_655 4_655 ?
Na2 P3 O1 156.27(17) 7_654 4_655 ?
Na3 P3 O1 106.53(14) . 4_655 ?
Na3 P3 O1 44.40(12) 1_554 4_655 ?
Na3 P3 O1 83.31(17) 8_544 4_655 ?
Na2 P3 O1 112.30(13) 1_654 4_655 ?
O7 P3 O7 65.39(16) . 8_545 ?
O8 P3 O7 77.8(3) . 8_545 ?
O6 P3 O7 166.2(3) 1_654 8_545 ?
O4 P3 O7 61.8(3) 6 8_545 ?
O1 P3 O7 111.16(16) 1_655 8_545 ?
Na2 P3 O7 40.38(13) 7_654 8_545 ?
Na3 P3 O7 42.05(14) . 8_545 ?
Na3 P3 O7 149.01(16) 1_554 8_545 ?
Na3 P3 O7 63.18(13) 8_544 8_545 ?
Na2 P3 O7 92.92(14) 1_654 8_545 ?
O1 P3 O7 130.6(2) 4_655 8_545 ?
O3 Na1 O3 140.01(19) 3_566 1_455 ?
O3 Na1 O3 140.01(19) 3_566 2_655 ?
O3 Na1 O3 57.8(3) 1_455 2_655 ?
O3 Na1 O3 57.8(3) 3_566 4_546 ?
O3 Na1 O3 140.0(2) 1_455 4_546 ?
O3 Na1 O3 140.0(2) 2_655 4_546 ?
O3 Na1 O5 55.21(17) 3_566 6_456 ?
O3 Na1 O5 89.68(18) 1_455 6_456 ?
O3 Na1 O5 102.18(18) 2_655 6_456 ?
O3 Na1 O5 111.42(17) 4_546 6_456 ?
O3 Na1 O5 111.42(17) 3_566 5_546 ?
O3 Na1 O5 102.18(18) 1_455 5_546 ?
O3 Na1 O5 89.68(18) 2_655 5_546 ?
O3 Na1 O5 55.21(17) 4_546 5_546 ?
O5 Na1 O5 166.53(16) 6_456 5_546 ?
O3 Na1 O5 102.18(18) 3_566 8_444 ?
O3 Na1 O5 55.21(17) 1_455 8_444 ?
O3 Na1 O5 111.42(17) 2_655 8_444 ?
O3 Na1 O5 89.68(18) 4_546 8_444 ?
O5 Na1 O5 90.788(19) 6_456 8_444 ?
O5 Na1 O5 90.788(19) 5_546 8_444 ?
O3 Na1 O5 89.68(18) 3_566 7_554 ?
O3 Na1 O5 111.42(17) 1_455 7_554 ?
O3 Na1 O5 55.21(17) 2_655 7_554 ?
O3 Na1 O5 102.18(18) 4_546 7_554 ?
O5 Na1 O5 90.79(2) 6_456 7_554 ?
O5 Na1 O5 90.788(19) 5_546 7_554 ?
O5 Na1 O5 166.53(16) 8_444 7_554 ?
O3 Na1 P1 151.08(15) 3_566 . ?
O3 Na1 P1 28.92(15) 1_455 . ?
O3 Na1 P1 28.92(15) 2_655 . ?
O3 Na1 P1 151.08(15) 4_546 . ?
O5 Na1 P1 96.73(8) 6_456 . ?
O5 Na1 P1 96.73(8) 5_546 . ?
O5 Na1 P1 83.27(8) 8_444 . ?
O5 Na1 P1 83.27(8) 7_554 . ?
O3 Na1 P1 28.92(15) 3_566 1_556 ?
O3 Na1 P1 151.08(15) 1_455 1_556 ?
O3 Na1 P1 151.08(15) 2_655 1_556 ?
O3 Na1 P1 28.92(15) 4_546 1_556 ?
O5 Na1 P1 83.27(8) 6_456 1_556 ?
O5 Na1 P1 83.27(8) 5_546 1_556 ?
O5 Na1 P1 96.73(8) 8_444 1_556 ?
O5 Na1 P1 96.73(8) 7_554 1_556 ?
P1 Na1 P1 180.0 . 1_556 ?
O3 Na1 O1 93.95(18) 3_566 . ?
O3 Na1 O1 61.83(18) 1_455 . ?
O3 Na1 O1 61.44(18) 2_655 . ?
O3 Na1 O1 151.79(17) 4_546 . ?
O5 Na1 O1 41.62(13) 6_456 . ?
O5 Na1 O1 151.03(13) 5_546 . ?
O5 Na1 O1 97.50(17) 8_444 . ?
O5 Na1 O1 75.06(17) 7_554 . ?
P1 Na1 O1 57.13(9) . . ?
P1 Na1 O1 122.87(9) 1_556 . ?
O3 Na1 O1 151.79(17) 3_566 2 ?
O3 Na1 O1 61.44(18) 1_455 2 ?
O3 Na1 O1 61.83(18) 2_655 2 ?
O3 Na1 O1 93.95(18) 4_546 2 ?
O5 Na1 O1 151.03(13) 6_456 2 ?
O5 Na1 O1 41.62(13) 5_546 2 ?
O5 Na1 O1 75.06(17) 8_444 2 ?
O5 Na1 O1 97.50(17) 7_554 2 ?
P1 Na1 O1 57.13(9) . 2 ?
P1 Na1 O1 122.87(9) 1_556 2 ?
O1 Na1 O1 114.26(17) . 2 ?
O7 Na2 O7 97.0(3) 2_666 1_456 ?
O7 Na2 O7 166.5(3) 2_666 8_445 ?
O7 Na2 O7 85.5(3) 1_456 8_445 ?
O7 Na2 O7 85.5(3) 2_666 7_565 ?
O7 Na2 O7 166.5(3) 1_456 7_565 ?
O7 Na2 O7 95.0(3) 8_445 7_565 ?
O7 Na2 O4 111.2(2) 2_666 4_556 ?
O7 Na2 O4 74.6(2) 1_456 4_556 ?
O7 Na2 O4 56.7(2) 8_445 4_556 ?
O7 Na2 O4 116.8(2) 7_565 4_556 ?
O7 Na2 O4 74.6(2) 2_666 3_566 ?
O7 Na2 O4 111.2(2) 1_456 3_566 ?
O7 Na2 O4 116.8(2) 8_445 3_566 ?
O7 Na2 O4 56.7(2) 7_565 3_566 ?
O4 Na2 O4 171.7(3) 4_556 3_566 ?
O7 Na2 Na2 131.48(16) 2_666 7_554 ?
O7 Na2 Na2 131.48(16) 1_456 7_554 ?
O7 Na2 Na2 47.52(16) 8_445 7_554 ?
O7 Na2 Na2 47.52(16) 7_565 7_554 ?
O4 Na2 Na2 85.83(13) 4_556 7_554 ?
O4 Na2 Na2 85.83(13) 3_566 7_554 ?
O7 Na2 Na2 48.52(16) 2_666 7 ?
O7 Na2 Na2 48.52(16) 1_456 7 ?
O7 Na2 Na2 132.48(16) 8_445 7 ?
O7 Na2 Na2 132.48(16) 7_565 7 ?
O4 Na2 Na2 94.17(13) 4_556 7 ?
O4 Na2 Na2 94.17(13) 3_566 7 ?
Na2 Na2 Na2 180.0 7_554 7 ?
O7 Na2 P3 141.73(19) 2_666 8_445 ?
O7 Na2 P3 77.28(17) 1_456 8_445 ?
O7 Na2 P3 26.20(16) 8_445 8_445 ?
O7 Na2 P3 108.7(2) 7_565 8_445 ?
O4 Na2 P3 30.59(13) 4_556 8_445 ?
O4 Na2 P3 143.01(19) 3_566 8_445 ?
Na2 Na2 P3 64.76(8) 7_554 8_445 ?
Na2 Na2 P3 115.24(8) 7 8_445 ?
O7 Na2 P3 77.28(17) 2_666 7_565 ?
O7 Na2 P3 141.73(19) 1_456 7_565 ?
O7 Na2 P3 108.7(2) 8_445 7_565 ?
O7 Na2 P3 26.20(16) 7_565 7_565 ?
O4 Na2 P3 143.01(19) 4_556 7_565 ?
O4 Na2 P3 30.59(13) 3_566 7_565 ?
Na2 Na2 P3 64.76(8) 7_554 7_565 ?
Na2 Na2 P3 115.24(8) 7 7_565 ?
P3 Na2 P3 129.51(16) 8_445 7_565 ?
O7 Na2 P3 21.50(18) 2_666 2_666 ?
O7 Na2 P3 103.48(19) 1_456 2_666 ?
O7 Na2 P3 145.15(18) 8_445 2_666 ?
O7 Na2 P3 83.71(17) 7_565 2_666 ?
O4 Na2 P3 92.84(15) 4_556 2_666 ?
O4 Na2 P3 91.55(17) 3_566 2_666 ?
Na2 Na2 P3 121.76(7) 7_554 2_666 ?
Na2 Na2 P3 58.24(7) 7 2_666 ?
P3 Na2 P3 122.38(9) 8_445 2_666 ?
P3 Na2 P3 85.04(8) 7_565 2_666 ?
O7 Na2 P3 103.48(19) 2_666 1_456 ?
O7 Na2 P3 21.50(18) 1_456 1_456 ?
O7 Na2 P3 83.71(17) 8_445 1_456 ?
O7 Na2 P3 145.15(18) 7_565 1_456 ?
O4 Na2 P3 91.55(17) 4_556 1_456 ?
O4 Na2 P3 92.84(15) 3_566 1_456 ?
Na2 Na2 P3 121.76(7) 7_554 1_456 ?
Na2 Na2 P3 58.24(7) 7 1_456 ?
P3 Na2 P3 85.04(8) 8_445 1_456 ?
P3 Na2 P3 122.38(9) 7_565 1_456 ?
P3 Na2 P3 116.48(14) 2_666 1_456 ?
O6 Na3 O7 98.4(2) 1_655 8_545 ?
O6 Na3 O1 78.0(2) 1_655 4_656 ?
O7 Na3 O1 131.0(3) 8_545 4_656 ?
O6 Na3 O8 159.4(3) 1_655 . ?
O7 Na3 O8 89.5(3) 8_545 . ?
O1 Na3 O8 110.8(3) 4_656 . ?
O6 Na3 O5 65.7(3) 1_655 6_556 ?
O7 Na3 O5 116.6(3) 8_545 6_556 ?
O1 Na3 O5 106.3(3) 4_656 6_556 ?
O8 Na3 O5 93.7(3) . 6_556 ?
O6 Na3 O4 107.0(3) 1_655 6 ?
O7 Na3 O4 74.6(2) 8_545 6 ?
O1 Na3 O4 153.8(3) 4_656 6 ?
O8 Na3 O4 56.8(3) . 6 ?
O5 Na3 O4 56.2(2) 6_556 6 ?
O6 Na3 P2 108.1(2) 1_655 8_545 ?
O7 Na3 P2 123.4(3) 8_545 8_545 ?
O1 Na3 P2 30.09(15) 4_656 8_545 ?
O8 Na3 P2 82.6(2) . 8_545 ?
O5 Na3 P2 119.8(2) 6_556 8_545 ?
O4 Na3 P2 136.8(2) 6 8_545 ?
O6 Na3 O5 122.8(3) 1_655 8_544 ?
O7 Na3 O5 133.7(3) 8_545 8_544 ?
O1 Na3 O5 51.80(18) 4_656 8_544 ?
O8 Na3 O5 59.8(2) . 8_544 ?
O5 Na3 O5 100.4(3) 6_556 8_544 ?
O4 Na3 O5 108.3(2) 6 8_544 ?
P2 Na3 O5 29.38(13) 8_545 8_544 ?
O6 Na3 O8 105.1(2) 1_655 8_545 ?
O7 Na3 O8 51.5(3) 8_545 8_545 ?
O1 Na3 O8 81.8(2) 4_656 8_545 ?
O8 Na3 O8 94.8(3) . 8_545 ?
O5 Na3 O8 165.2(3) 6_556 8_545 ?
O4 Na3 O8 120.0(3) 6 8_545 ?
P2 Na3 O8 73.32(19) 8_545 8_545 ?
O5 Na3 O8 94.3(3) 8_544 8_545 ?
O6 Na3 P3 137.3(3) 1_655 . ?
O7 Na3 P3 75.61(15) 8_545 . ?
O1 Na3 P3 137.5(2) 4_656 . ?
O8 Na3 P3 27.6(2) . . ?
O5 Na3 P3 79.19(15) 6_556 . ?
O4 Na3 P3 30.29(14) 6 . ?
P2 Na3 P3 110.20(12) 8_545 . ?
O5 Na3 P3 85.73(13) 8_544 . ?
O8 Na3 P3 103.37(16) 8_545 . ?
O6 Na3 P3 24.91(19) 1_655 1_556 ?
O7 Na3 P3 85.14(15) 8_545 1_556 ?
O1 Na3 P3 71.49(15) 4_656 1_556 ?
O8 Na3 P3 174.3(3) . 1_556 ?
O5 Na3 P3 90.51(16) 6_556 1_556 ?
O4 Na3 P3 123.4(2) 6 1_556 ?
P2 Na3 P3 98.60(12) 8_545 1_556 ?
O5 Na3 P3 123.12(16) 8_544 1_556 ?
O8 Na3 P3 80.29(14) 8_545 1_556 ?
P3 Na3 P3 150.87(17) . 1_556 ?
O6 Na3 P2 86.0(2) 1_655 6 ?
O7 Na3 P2 97.3(2) 8_545 6 ?
O1 Na3 P2 130.6(3) 4_656 6 ?
O8 Na3 P2 74.1(2) . 6 ?
O5 Na3 P2 27.13(13) 6_556 6 ?
O4 Na3 P2 29.15(16) 6 6 ?
P2 Na3 P2 132.80(18) 8_545 6 ?
O5 Na3 P2 105.21(17) 8_544 6 ?
O8 Na3 P2 147.6(2) 8_545 6 ?
P3 Na3 P2 53.91(9) . 6 ?
P3 Na3 P2 108.61(13) 1_556 6 ?
P2 O1 Al1 130.3(5) 6_455 3_565 ?
P2 O1 V1 130.3(5) 6_455 3_565 ?
Al1 O1 V1 0.0 3_565 3_565 ?
P2 O1 O5 35.9(2) 6_455 6_456 ?
Al1 O1 O5 155.2(4) 3_565 6_456 ?
V1 O1 O5 155.2(4) 3_565 6_456 ?
P2 O1 O2 31.7(2) 6_455 6_455 ?
Al1 O1 O2 119.1(4) 3_565 6_455 ?
V1 O1 O2 119.1(4) 3_565 6_455 ?
O5 O1 O2 60.5(3) 6_456 6_455 ?
P2 O1 O4 37.1(2) 6_455 6_455 ?
Al1 O1 O4 98.2(3) 3_565 6_455 ?
V1 O1 O4 98.2(3) 3_565 6_455 ?
O5 O1 O4 59.7(3) 6_456 6_455 ?
O2 O1 O4 57.4(3) 6_455 6_455 ?
P2 O1 Na3 91.9(3) 6_455 3_566 ?
Al1 O1 Na3 130.8(3) 3_565 3_566 ?
V1 O1 Na3 130.8(3) 3_565 3_566 ?
O5 O1 Na3 73.9(2) 6_456 3_566 ?
O2 O1 Na3 82.0(3) 6_455 3_566 ?
O4 O1 Na3 128.5(2) 6_455 3_566 ?
P2 O1 O2 94.5(4) 6_455 3_565 ?
Al1 O1 O2 45.4(2) 3_565 3_565 ?
V1 O1 O2 45.4(2) 3_565 3_565 ?
O5 O1 O2 130.4(4) 6_456 3_565 ?
O2 O1 O2 74.3(2) 6_455 3_565 ?
O4 O1 O2 79.8(3) 6_455 3_565 ?
Na3 O1 O2 120.9(4) 3_566 3_565 ?
P2 O1 O6 93.2(4) 6_455 1_554 ?
Al1 O1 O6 45.00(19) 3_565 1_554 ?
V1 O1 O6 45.00(19) 3_565 1_554 ?
O5 O1 O6 110.2(3) 6_456 1_554 ?
O2 O1 O6 102.6(3) 6_455 1_554 ?
O4 O1 O6 56.5(2) 6_455 1_554 ?
Na3 O1 O6 174.9(3) 3_566 1_554 ?
O2 O1 O6 59.1(2) 3_565 1_554 ?
P2 O1 O3 146.8(5) 6_455 3_565 ?
Al1 O1 O3 42.44(18) 3_565 3_565 ?
V1 O1 O3 42.44(18) 3_565 3_565 ?
O5 O1 O3 131.5(4) 6_456 3_565 ?
O2 O1 O3 160.2(4) 6_455 3_565 ?
O4 O1 O3 111.9(3) 6_455 3_565 ?
Na3 O1 O3 115.1(3) 3_566 3_565 ?
O2 O1 O3 87.8(2) 3_565 3_565 ?
O6 O1 O3 59.9(2) 1_554 3_565 ?
P2 O1 O8 146.1(5) 6_455 3_565 ?
Al1 O1 O8 42.26(19) 3_565 3_565 ?
V1 O1 O8 42.26(19) 3_565 3_565 ?
O5 O1 O8 162.6(4) 6_456 3_565 ?
O2 O1 O8 115.5(4) 6_455 3_565 ?
O4 O1 O8 134.7(3) 6_455 3_565 ?
Na3 O1 O8 88.8(3) 3_566 3_565 ?
O2 O1 O8 57.0(3) 3_565 3_565 ?
O6 O1 O8 87.2(2) 1_554 3_565 ?
O3 O1 O8 58.2(2) 3_565 3_565 ?
P2 O1 O6 139.7(4) 6_455 3_556 ?
Al1 O1 O6 86.2(2) 3_565 3_556 ?
V1 O1 O6 86.2(2) 3_565 3_556 ?
O5 O1 O6 115.7(3) 6_456 3_556 ?
O2 O1 O6 121.9(4) 6_455 3_556 ?
O4 O1 O6 175.3(3) 6_455 3_556 ?
Na3 O1 O6 47.85(19) 3_566 3_556 ?
O2 O1 O6 104.7(3) 3_565 3_556 ?
O6 O1 O6 127.1(3) 1_554 3_556 ?
O3 O1 O6 70.2(2) 3_565 3_556 ?
O8 O1 O6 50.0(2) 3_565 3_556 ?
P2 O2 V1 165.7(4) . . ?
P2 O2 O4 40.1(3) . . ?
V1 O2 O4 143.2(4) . . ?
P2 O2 O5 33.6(2) . 1_554 ?
V1 O2 O5 154.5(3) . 1_554 ?
O4 O2 O5 60.4(3) . 1_554 ?
P2 O2 O1 32.5(2) . 6 ?
V1 O2 O1 133.2(4) . 6 ?
O4 O2 O1 61.5(3) . 6 ?
O5 O2 O1 58.6(3) 1_554 6 ?
P2 O2 O8 121.7(5) . . ?
V1 O2 O8 47.1(3) . . ?
O4 O2 O8 149.7(3) . . ?
O5 O2 O8 120.7(4) 1_554 . ?
O1 O2 O8 92.3(3) 6 . ?
P2 O2 O1 141.8(4) . 4_655 ?
V1 O2 O1 47.8(2) . 4_655 ?
O4 O2 O1 144.5(3) . 4_655 ?
O5 O2 O1 108.4(3) 1_554 4_655 ?
O1 O2 O1 145.3(4) 6 4_655 ?
O8 O2 O1 65.8(3) . 4_655 ?
P2 O2 O6 142.1(5) . 4_656 ?
V1 O2 O6 46.7(2) . 4_656 ?
O4 O2 O6 102.2(4) . 4_656 ?
O5 O2 O6 137.9(3) 1_554 4_656 ?
O1 O2 O6 150.3(3) 6 4_656 ?
O8 O2 O6 93.7(3) . 4_656 ?
O1 O2 O6 62.0(2) 4_655 4_656 ?
P2 O2 O5 126.5(3) . 8_544 ?
V1 O2 O5 43.01(18) . 8_544 ?
O4 O2 O5 107.7(3) . 8_544 ?
O5 O2 O5 159.7(3) 1_554 8_544 ?
O1 O2 O5 101.6(3) 6 8_544 ?
O8 O2 O5 60.2(2) . 8_544 ?
O1 O2 O5 90.7(3) 4_655 8_544 ?
O6 O2 O5 57.5(2) 4_656 8_544 ?
P2 O2 O2 77.8(3) . 8_545 ?
V1 O2 O2 90.4(3) . 8_545 ?
O4 O2 O2 72.5(2) . 8_545 ?
O5 O2 O2 110.8(4) 1_554 8_545 ?
O1 O2 O2 55.1(2) 6 8_545 ?
O8 O2 O2 80.15(18) . 8_545 ?
O1 O2 O2 137.4(4) 4_655 8_545 ?
O6 O2 O2 97.4(3) 4_656 8_545 ?
O5 O2 O2 48.9(2) 8_544 8_545 ?
P2 O2 O2 93.7(4) . 8_544 ?
V1 O2 O2 98.0(3) . 8_544 ?
O4 O2 O2 101.5(3) . 8_544 ?
O5 O2 O2 60.6(2) 1_554 8_544 ?
O1 O2 O2 116.7(4) 6 8_544 ?
O8 O2 O2 104.1(2) . 8_544 ?
O1 O2 O2 50.6(2) 4_655 8_544 ?
O6 O2 O2 89.9(2) 4_656 8_544 ?
O5 O2 O2 139.7(4) 8_544 8_544 ?
O2 O2 O2 171.4(5) 8_545 8_544 ?
P1 O3 V1 138.9(3) 1_655 . ?
P1 O3 O3 37.5(2) 1_655 2_755 ?
V1 O3 O3 171.8(5) . 2_755 ?
P1 O3 Na1 98.6(3) 1_655 1_655 ?
V1 O3 Na1 121.6(2) . 1_655 ?
O3 O3 Na1 61.08(15) 2_755 1_655 ?
P1 O3 O3 34.13(11) 1_655 3_665 ?
V1 O3 O3 120.0(4) . 3_665 ?
O3 O3 O3 61.36(13) 2_755 3_665 ?
Na1 O3 O3 114.3(3) 1_655 3_665 ?
P1 O3 O3 34.13(11) 1_655 4_645 ?
V1 O3 O3 111.9(4) . 4_645 ?
O3 O3 O3 61.36(13) 2_755 4_645 ?
Na1 O3 O3 114.3(3) 1_655 4_645 ?
O3 O3 O3 57.3(3) 3_665 4_645 ?
P1 O3 O5 162.3(4) 1_655 8_544 ?
V1 O3 O5 49.3(2) . 8_544 ?
O3 O3 O5 131.3(3) 2_755 8_544 ?
Na1 O3 O5 72.7(2) 1_655 8_544 ?
O3 O3 O5 163.6(4) 3_665 8_544 ?
O3 O3 O5 135.2(4) 4_645 8_544 ?
P1 O3 O8 135.0(3) 1_655 . ?
V1 O3 O8 45.0(3) . . ?
O3 O3 O8 143.1(5) 2_755 . ?
Na1 O3 O8 106.4(2) 1_655 . ?
O3 O3 O8 100.9(3) 3_665 . ?
O3 O3 O8 138.9(3) 4_645 . ?
O5 O3 O8 62.7(3) 8_544 . ?
P1 O3 O6 113.1(3) 1_655 4_656 ?
V1 O3 O6 44.7(2) . 4_656 ?
O3 O3 O6 127.3(4) 2_755 4_656 ?
Na1 O3 O6 114.7(2) 1_655 4_656 ?
O3 O3 O6 124.0(3) 3_665 4_656 ?
O3 O3 O6 79.0(3) 4_645 4_656 ?
O5 O3 O6 59.9(2) 8_544 4_656 ?
O8 O3 O6 89.6(3) . 4_656 ?
P1 O3 O1 94.8(3) 1_655 4_655 ?
V1 O3 O1 45.29(18) . 4_655 ?
O3 O3 O1 132.33(19) 2_755 4_655 ?
Na1 O3 O1 166.6(3) 1_655 4_655 ?
O3 O3 O1 77.0(3) 3_665 4_655 ?
O3 O3 O1 77.5(3) 4_645 4_655 ?
O5 O3 O1 94.5(3) 8_544 4_655 ?
O8 O3 O1 63.0(2) . 4_655 ?
O6 O3 O1 59.5(2) 4_656 4_655 ?
P1 O3 O1 75.6(3) 1_655 2_655 ?
V1 O3 O1 103.6(3) . 2_655 ?
O3 O3 O1 69.0(3) 2_755 2_655 ?
Na1 O3 O1 76.94(18) 1_655 2_655 ?
O3 O3 O1 108.6(2) 3_665 2_655 ?
O3 O3 O1 55.0(2) 4_645 2_655 ?
O5 O3 O1 87.3(3) 8_544 2_655 ?
O8 O3 O1 145.9(3) . 2_655 ?
O6 O3 O1 59.8(2) 4_656 2_655 ?
O1 O3 O1 107.1(2) 4_655 2_655 ?
P2 O4 P3 131.1(5) . 6_455 ?
P2 O4 O2 36.1(3) . . ?
P3 O4 O2 148.2(4) 6_455 . ?
P2 O4 O7 159.7(4) . 6_455 ?
P3 O4 O7 36.3(2) 6_455 6_455 ?
O2 O4 O7 140.0(4) . 6_455 ?
P2 O4 O8 119.6(5) . 6_455 ?
P3 O4 O8 36.0(2) 6_455 6_455 ?
O2 O4 O8 155.6(4) . 6_455 ?
O7 O4 O8 61.0(3) 6_455 6_455 ?
P2 O4 O5 36.4(2) . 1_554 ?
P3 O4 O5 129.7(5) 6_455 1_554 ?
O2 O4 O5 61.6(3) . 1_554 ?
O7 O4 O5 158.3(5) 6_455 1_554 ?
O8 O4 O5 98.9(4) 6_455 1_554 ?
P2 O4 O6 100.4(3) . 6_556 ?
P3 O4 O6 35.5(2) 6_455 6_556 ?
O2 O4 O6 113.4(3) . 6_556 ?
O7 O4 O6 61.1(3) 6_455 6_556 ?
O8 O4 O6 61.0(2) 6_455 6_556 ?
O5 O4 O6 118.3(4) 1_554 6_556 ?
P2 O4 O1 34.3(2) . 6 ?
P3 O4 O1 97.3(3) 6_455 6 ?
O2 O4 O1 61.1(3) . 6 ?
O7 O4 O1 127.4(3) 6_455 6 ?
O8 O4 O1 97.1(4) 6_455 6 ?
O5 O4 O1 58.9(2) 1_554 6 ?
O6 O4 O1 66.4(3) 6_556 6 ?
P2 O4 Na3 97.3(3) . 6_455 ?
P3 O4 Na3 93.6(4) 6_455 6_455 ?
O2 O4 Na3 114.8(3) . 6_455 ?
O7 O4 Na3 99.4(3) 6_455 6_455 ?
O8 O4 Na3 59.5(2) 6_455 6_455 ?
O5 O4 Na3 60.9(3) 1_554 6_455 ?
O6 O4 Na3 119.1(3) 6_556 6_455 ?
O1 O4 Na3 109.0(3) 6 6_455 ?
P2 O4 Na2 135.5(4) . 3_556 ?
P3 O4 Na2 90.0(3) 6_455 3_556 ?
O2 O4 Na2 100.5(3) . 3_556 ?
O7 O4 Na2 53.9(2) 6_455 3_556 ?
O8 O4 Na2 103.6(3) 6_455 3_556 ?
O5 O4 Na2 131.9(3) 1_554 3_556 ?
O6 O4 Na2 109.8(3) 6_556 3_556 ?
O1 O4 Na2 153.6(4) 6 3_556 ?
Na3 O4 Na2 95.7(2) 6_455 3_556 ?
P2 O4 O7 131.1(3) . 3_565 ?
P3 O4 O7 90.7(3) 6_455 3_565 ?
O2 O4 O7 118.3(3) . 3_565 ?
O7 O4 O7 69.22(17) 6_455 3_565 ?
O8 O4 O7 77.3(3) 6_455 3_565 ?
O5 O4 O7 100.0(2) 1_554 3_565 ?
O6 O4 O7 125.8(3) 6_556 3_565 ?
O1 O4 O7 157.4(3) 6 3_565 ?
Na3 O4 O7 49.2(2) 6_455 3_565 ?
Na2 O4 O7 46.62(18) 3_556 3_565 ?
P2 O4 O2 70.0(3) . 8_545 ?
P3 O4 O2 84.7(3) 6_455 8_545 ?
O2 O4 O2 63.7(2) . 8_545 ?
O7 O4 O2 90.8(2) 6_455 8_545 ?
O8 O4 O2 112.9(2) 6_455 8_545 ?
O5 O4 O2 105.5(3) 1_554 8_545 ?
O6 O4 O2 52.3(2) 6_556 8_545 ?
O1 O4 O2 52.1(2) 6 8_545 ?
Na3 O4 O2 160.3(4) 6_455 8_545 ?
Na2 O4 O2 103.9(3) 3_556 8_545 ?
O7 O4 O2 150.2(3) 3_565 8_545 ?
P2 O5 V1 141.5(5) 1_556 8_545 ?
P2 O5 Al1 141.5(5) 1_556 8_545 ?
V1 O5 Al1 0.00(2) 8_545 8_545 ?
P2 O5 O1 35.3(2) 1_556 6_556 ?
V1 O5 O1 149.9(4) 8_545 6_556 ?
Al1 O5 O1 149.9(4) 8_545 6_556 ?
P2 O5 O4 38.7(3) 1_556 1_556 ?
V1 O5 O4 140.8(4) 8_545 1_556 ?
Al1 O5 O4 140.8(4) 8_545 1_556 ?
O1 O5 O4 61.5(2) 6_556 1_556 ?
P2 O5 O2 32.3(2) 1_556 1_556 ?
V1 O5 O2 109.3(4) 8_545 1_556 ?
Al1 O5 O2 109.3(4) 8_545 1_556 ?
O1 O5 O2 60.8(2) 6_556 1_556 ?
O4 O5 O2 58.0(3) 1_556 1_556 ?
P2 O5 Na3 101.5(4) 1_556 6_456 ?
V1 O5 Na3 97.4(3) 8_545 6_456 ?
Al1 O5 Na3 97.4(3) 8_545 6_456 ?
O1 O5 Na3 112.7(3) 6_556 6_456 ?
O4 O5 Na3 62.8(2) 1_556 6_456 ?
O2 O5 Na3 113.4(3) 1_556 6_456 ?
P2 O5 O3 164.6(5) 1_556 8_545 ?
V1 O5 O3 45.89(18) 8_545 8_545 ?
Al1 O5 O3 45.89(18) 8_545 8_545 ?
O1 O5 O3 129.9(4) 6_556 8_545 ?
O4 O5 O3 150.2(4) 1_556 8_545 ?
O2 O5 O3 150.5(4) 1_556 8_545 ?
Na3 O5 O3 88.8(3) 6_456 8_545 ?
P2 O5 O6 132.4(5) 1_556 6_556 ?
V1 O5 O6 46.37(19) 8_545 6_556 ?
Al1 O5 O6 46.37(19) 8_545 6_556 ?
O1 O5 O6 162.8(4) 6_556 6_556 ?
O4 O5 O6 101.7(3) 1_556 6_556 ?
O2 O5 O6 114.7(4) 1_556 6_556 ?
Na3 O5 O6 52.1(2) 6_456 6_556 ?
O3 O5 O6 63.0(2) 8_545 6_556 ?
P2 O5 O8 113.2(4) 1_556 8_545 ?
V1 O5 O8 44.4(2) 8_545 8_545 ?
Al1 O5 O8 44.4(2) 8_545 8_545 ?
O1 O5 O8 105.6(3) 6_556 8_545 ?
O4 O5 O8 147.8(4) 1_556 8_545 ?
O2 O5 O8 89.8(3) 1_556 8_545 ?
Na3 O5 O8 141.3(2) 6_456 8_545 ?
O3 O5 O8 61.4(3) 8_545 8_545 ?
O6 O5 O8 90.6(2) 6_556 8_545 ?
P2 O5 O2 102.1(4) 1_556 8_545 ?
V1 O5 O2 40.8(2) 8_545 8_545 ?
Al1 O5 O2 40.8(2) 8_545 8_545 ?
O1 O5 O2 128.1(4) 6_556 8_545 ?
O4 O5 O2 106.8(3) 1_556 8_545 ?
O2 O5 O2 70.5(2) 1_556 8_545 ?
Na3 O5 O2 101.7(3) 6_456 8_545 ?
O3 O5 O2 86.7(2) 8_545 8_545 ?
O6 O5 O2 57.1(2) 6_556 8_545 ?
O8 O5 O2 55.8(3) 8_545 8_545 ?
P2 O5 Na3 74.9(3) 1_556 8_545 ?
V1 O5 Na3 96.1(3) 8_545 8_545 ?
Al1 O5 Na3 96.1(3) 8_545 8_545 ?
O1 O5 Na3 54.3(2) 6_556 8_545 ?
O4 O5 Na3 112.2(2) 1_556 8_545 ?
O2 O5 Na3 73.3(3) 1_556 8_545 ?
Na3 O5 Na3 161.7(3) 6_456 8_545 ?
O3 O5 Na3 91.7(3) 8_545 8_545 ?
O6 O5 Na3 142.5(3) 6_556 8_545 ?
O8 O5 Na3 52.0(2) 8_545 8_545 ?
O2 O5 Na3 96.6(3) 8_545 8_545 ?
P3 O6 Al1 136.4(4) 1_456 3_566 ?
P3 O6 V1 136.4(4) 1_456 3_566 ?
Al1 O6 V1 0.0 3_566 3_566 ?
P3 O6 Na3 114.8(4) 1_456 1_455 ?
Al1 O6 Na3 108.4(3) 3_566 1_455 ?
V1 O6 Na3 108.4(3) 3_566 1_455 ?
P3 O6 O4 38.1(2) 1_456 6_456 ?
Al1 O6 O4 99.6(3) 3_566 6_456 ?
V1 O6 O4 99.6(3) 3_566 6_456 ?
Na3 O6 O4 151.6(4) 1_455 6_456 ?
P3 O6 O7 32.6(2) 1_456 1_456 ?
Al1 O6 O7 149.5(4) 3_566 1_456 ?
V1 O6 O7 149.5(4) 3_566 1_456 ?
Na3 O6 O7 94.2(3) 1_455 1_456 ?
O4 O6 O7 58.0(2) 6_456 1_456 ?
P3 O6 O8 33.0(3) 1_456 1_456 ?
Al1 O6 O8 130.3(4) 3_566 1_456 ?
V1 O6 O8 130.3(4) 3_566 1_456 ?
Na3 O6 O8 103.6(4) 1_455 1_456 ?
O4 O6 O8 58.9(3) 6_456 1_456 ?
O7 O6 O8 59.2(3) 1_456 1_456 ?
P3 O6 O2 113.6(4) 1_456 3_566 ?
Al1 O6 O2 45.3(2) 3_566 3_566 ?
V1 O6 O2 45.3(2) 3_566 3_566 ?
Na3 O6 O2 117.1(3) 1_455 3_566 ?
O4 O6 O2 80.0(3) 6_456 3_566 ?
O7 O6 O2 106.3(3) 1_456 3_566 ?
O8 O6 O2 138.2(3) 1_456 3_566 ?
P3 O6 O5 173.9(4) 1_456 6_456 ?
Al1 O6 O5 47.6(2) 3_566 6_456 ?
V1 O6 O5 47.6(2) 3_566 6_456 ?
Na3 O6 O5 62.2(2) 1_455 6_456 ?
O4 O6 O5 143.5(4) 6_456 6_456 ?
O7 O6 O5 141.3(3) 1_456 6_456 ?
O8 O6 O5 151.0(4) 1_456 6_456 ?
O2 O6 O5 65.4(3) 3_566 6_456 ?
P3 O6 O1 90.8(3) 1_456 1_556 ?
Al1 O6 O1 45.96(19) 3_566 1_556 ?
V1 O6 O1 45.96(19) 3_566 1_556 ?
Na3 O6 O1 150.7(4) 1_455 1_556 ?
O4 O6 O1 57.1(2) 6_456 1_556 ?
O7 O6 O1 115.0(3) 1_456 1_556 ?
O8 O6 O1 90.2(3) 1_456 1_556 ?
O2 O6 O1 58.9(2) 3_566 1_556 ?
O5 O6 O1 93.5(3) 6_456 1_556 ?
P3 O6 O3 128.9(4) 1_456 3_566 ?
Al1 O6 O3 42.8(2) 3_566 3_566 ?
V1 O6 O3 42.8(2) 3_566 3_566 ?
Na3 O6 O3 91.1(3) 1_455 3_566 ?
O4 O6 O3 113.1(3) 6_456 3_566 ?
O7 O6 O3 160.1(4) 1_456 3_566 ?
O8 O6 O3 100.9(3) 1_456 3_566 ?
O2 O6 O3 88.1(3) 3_566 3_566 ?
O5 O6 O3 57.1(2) 6_456 3_566 ?
O1 O6 O3 60.6(2) 1_556 3_566 ?
P3 O6 O1 90.9(4) 1_456 4_556 ?
Al1 O6 O1 110.8(3) 3_566 4_556 ?
V1 O6 O1 110.8(3) 3_566 4_556 ?
Na3 O6 O1 54.1(2) 1_455 4_556 ?
O4 O6 O1 119.5(3) 6_456 4_556 ?
O7 O6 O1 99.0(3) 1_456 4_556 ?
O8 O6 O1 61.5(3) 1_456 4_556 ?
O2 O6 O1 154.1(3) 3_566 4_556 ?
O5 O6 O1 91.2(3) 6_456 4_556 ?
O1 O6 O1 115.1(4) 1_556 4_556 ?
O3 O6 O1 69.0(3) 3_566 4_556 ?
P3 O7 Na2 123.5(4) . 1_654 ?
P3 O7 Na2 109.2(3) . 7_654 ?
Na2 O7 Na2 84.0(2) 1_654 7_654 ?
P3 O7 Na3 112.2(4) . 8_544 ?
Na2 O7 Na3 115.0(3) 1_654 8_544 ?
Na2 O7 Na3 107.8(3) 7_654 8_544 ?
P3 O7 O4 40.1(3) . 6 ?
Na2 O7 O4 114.4(4) 1_654 6 ?
Na2 O7 O4 69.4(2) 7_654 6 ?
Na3 O7 O4 129.8(3) 8_544 6 ?
P3 O7 O8 33.8(3) . . ?
Na2 O7 O8 152.6(3) 1_654 . ?
Na2 O7 O8 115.1(2) 7_654 . ?
Na3 O7 O8 79.2(3) 8_544 . ?
O4 O7 O8 60.3(4) 6 . ?
P3 O7 O6 33.5(2) . 1_654 ?
Na2 O7 O6 92.7(3) 1_654 1_654 ?
Na2 O7 O6 123.3(3) 7_654 1_654 ?
Na3 O7 O6 124.2(3) 8_544 1_654 ?
O4 O7 O6 60.9(3) 6 1_654 ?
O8 O7 O6 60.7(3) . 1_654 ?
P3 O7 O4 147.0(4) . 4_655 ?
Na2 O7 O4 58.8(2) 1_654 4_655 ?
Na2 O7 O4 103.8(3) 7_654 4_655 ?
Na3 O7 O4 56.3(2) 8_544 4_655 ?
O4 O7 O4 171.5(5) 6 4_655 ?
O8 O7 O4 128.1(4) . 4_655 ?
O6 O7 O4 122.3(2) 1_654 4_655 ?
P3 O7 O7 108.0(3) . 8_544 ?
Na2 O7 O7 47.72(16) 1_654 8_544 ?
Na2 O7 O7 130.2(2) 7_654 8_544 ?
Na3 O7 O7 87.0(2) 8_544 8_544 ?
O4 O7 O7 134.7(4) 6 8_544 ?
O8 O7 O7 114.3(2) . 8_544 ?
O6 O7 O7 77.3(2) 1_654 8_544 ?
O4 O7 O7 45.8(2) 4_655 8_544 ?
P3 O7 O7 89.5(3) . 8_545 ?
Na2 O7 O7 129.21(19) 1_654 8_545 ?
Na2 O7 O7 46.74(16) 7_654 8_545 ?
Na3 O7 O7 77.6(2) 8_544 8_545 ?
O4 O7 O7 65.0(2) 6 8_545 ?
O8 O7 O7 75.18(19) . 8_545 ?
O6 O7 O7 121.7(3) 1_654 8_545 ?
O4 O7 O7 114.4(3) 4_655 8_545 ?
O7 O7 O7 160.2(5) 8_544 8_545 ?
P3 O7 O7 126.5(5) . 2_765 ?
Na2 O7 O7 41.48(15) 1_654 2_765 ?
Na2 O7 O7 42.48(16) 7_654 2_765 ?
Na3 O7 O7 119.4(4) 8_544 2_765 ?
O4 O7 O7 92.7(3) 6 2_765 ?
O8 O7 O7 152.3(4) . 2_765 ?
O6 O7 O7 113.4(4) 1_654 2_765 ?
O4 O7 O7 78.8(3) 4_655 2_765 ?
O7 O7 O7 88.45(8) 8_544 2_765 ?
O7 O7 O7 88.45(8) 8_545 2_765 ?
P3 O7 P3 120.1(3) . 8_544 ?
Na2 O7 P3 62.34(13) 1_654 8_544 ?
Na2 O7 P3 129.9(3) 7_654 8_544 ?
Na3 O7 P3 62.33(16) 8_544 8_544 ?
O4 O7 P3 156.8(3) 6 8_544 ?
O8 O7 P3 110.9(3) . 8_544 ?
O6 O7 P3 95.91(19) 1_654 8_544 ?
O4 O7 P3 27.52(12) 4_655 8_544 ?
O7 O7 P3 25.13(15) 8_544 8_544 ?
O7 O7 P3 136.4(3) 8_545 8_544 ?
O7 O7 P3 96.41(18) 2_765 8_544 ?
P3 O8 V1 136.7(4) . . ?
P3 O8 O4 39.0(3) . 6 ?
V1 O8 O4 143.0(5) . 6 ?
P3 O8 O7 33.2(3) . . ?
V1 O8 O7 145.6(3) . . ?
O4 O8 O7 58.7(3) 6 . ?
P3 O8 O6 33.3(2) . 1_654 ?
V1 O8 O6 103.6(3) . 1_654 ?
O4 O8 O6 60.1(3) 6 1_654 ?
O7 O8 O6 60.1(3) . 1_654 ?
P3 O8 Na3 100.6(4) . . ?
V1 O8 Na3 113.2(3) . . ?
O4 O8 Na3 63.7(2) 6 . ?
O7 O8 Na3 100.7(3) . . ?
O6 O8 Na3 122.3(4) 1_654 . ?
P3 O8 O2 138.0(4) . . ?
V1 O8 O2 45.5(3) . . ?
O4 O8 O2 171.5(5) 6 . ?
O7 O8 O2 114.5(4) . . ?
O6 O8 O2 122.2(3) 1_654 . ?
Na3 O8 O2 115.3(3) . . ?
P3 O8 O3 107.8(4) . . ?
V1 O8 O3 42.8(2) . . ?
O4 O8 O3 100.1(4) 6 . ?
O7 O8 O3 139.1(4) . . ?
O6 O8 O3 79.1(3) 1_654 . ?
Na3 O8 O3 98.9(3) . . ?
O2 O8 O3 88.3(4) . . ?
P3 O8 O5 156.0(6) . 8_544 ?
V1 O8 O5 45.3(2) . 8_544 ?
O4 O8 O5 121.0(3) 6 8_544 ?
O7 O8 O5 164.3(3) . 8_544 ?
O6 O8 O5 135.0(4) 1_654 8_544 ?
Na3 O8 O5 68.2(2) . 8_544 ?
O2 O8 O5 64.0(3) . 8_544 ?
O3 O8 O5 55.9(3) . 8_544 ?
P3 O8 O1 97.9(3) . 4_655 ?
V1 O8 O1 42.93(19) . 4_655 ?
O4 O8 O1 127.5(3) 6 4_655 ?
O7 O8 O1 104.1(3) . 4_655 ?
O6 O8 O1 68.5(2) 1_654 4_655 ?
Na3 O8 O1 154.8(4) . 4_655 ?
O2 O8 O1 57.2(3) . 4_655 ?
O3 O8 O1 58.9(2) . 4_655 ?
O5 O8 O1 88.2(3) 8_544 4_655 ?
P3 O8 Na3 81.9(4) . 8_544 ?
V1 O8 Na3 113.5(4) . 8_544 ?
O4 O8 Na3 102.5(3) 6 8_544 ?
O7 O8 Na3 49.3(2) . 8_544 ?
O6 O8 Na3 100.1(3) 1_654 8_544 ?
Na3 O8 Na3 103.9(3) . 8_544 ?
O2 O8 Na3 69.3(3) . 8_544 ?
O3 O8 Na3 153.2(3) . 8_544 ?
O5 O8 Na3 120.8(3) 8_544 8_544 ?
O1 O8 Na3 95.6(3) 4_655 8_544 ?
 
_refine_diff_density_max    0.708
_refine_diff_density_min   -0.737
_refine_diff_density_rms    0.170
